HAL Id: hal-01634005
Submitted on 13 Nov 2017
HAL is a multi-disciplinary open access
archive for the deposit and dissemination of
sci-entific research documents, whether they are
pub-lished or not. The documents may come from
teaching and research institutions in France or
abroad, or from public or private research centers.
L’archive ouverte pluridisciplinaire HAL, est
destinée au dépôt et à la diffusion de documents
scientifiques de niveau recherche, publiés ou non,
émanant des établissements d’enseignement et de
recherche français ou étrangers, des laboratoires
publics ou privés.
Mouad Jebli, Frédéric Jamin, Etienne Malachanne, Eric Garcia-Diaz, Moulay
Saïd El Youssoufi
To cite this version:
Mouad Jebli, Frédéric Jamin, Etienne Malachanne, Eric Garcia-Diaz, Moulay Saïd El Youssoufi.
Experimental characterization of mechanical properties of the cement paste- aggregate interface in
concrete. Powders & Grains 2017, Jul 2017, Montpellier, France. �10.1051/epjconf/201714012014�.
Experimental characterization of mechanical properties of the cement
paste-aggregate interface in concrete
M. Jebli1,3,, F. Jamin1,3, E. Malachanne2, E. Garcia-Diaz2, and M.S. El Youssouﬁ1,3
1LMGC, Univ. Montpellier, CNRS, Montpellier, France 2C2MA, Ecole des mines d’Alès, Alès, France 3MIST Lab., IRSN, CNRS, Univ. Montpellier, France
Abstract. Granular materials are extensively used in the ﬁeld of civil engineering. These materials are either used in their dry state, or mixed with water or with a binder. In the case of concrete, the binder could be cement or mortar. For ordinary concretes, it is generally admitted that there is a thin heterogeneous zone of paste, with a thickness of about 15-60μm, surrounding the aggregates surface. This zone, commonly named the Interfacial Transition Zone (ITZ), is characterized by a higher porosity than the bulk paste and a high concentration of the portlandite crystals. Some of these crystals react with the aggregates’ surface (limestone aggregates), leading to a good adhesion. In this work, the mechanical properties of the cement paste and of the cement-aggregate interface are experimentally analyzed. Experimental tensile and shear tests are performed on parallelipipedic samples. These samples are made by linking limestone aggregates with Portland cement paste using a water/ cement ratio of 0.5. The results show that the cement-aggregate interface is the weak zone in the composite.
Concrete is a composite material of aggregate particles and cement paste. The mechanical properties of concrete de-pend on the properties of the cement paste, the aggregates and the cement paste-aggregate interface. The cement-aggregate interface is characterized by a higher porosity than that found in the bulk paste. For this reason, the me-chanical properties of this zone are considered diﬀerent than those of the cement paste.
There is ample evidence that the properties of concrete, such as the tensile strength, modes of failure and the per-meability; are signiﬁcantly inﬂuenced by the nature of the existing interfaces between the cement paste and the ag-gregates. However, due to lack of understanding about these interfaces, very little attempts have been made to characterize the mechanical properties of this zone. Some studies have been devoted to the direct characterization of the mechanical properties of the interface between aggre-gates and cement paste, by using tensile and shear tests.
The literature of bond strength prior to 1965 has been admirably reviewed by Alexander et al.  and by Shah and Slate . Both papers support the ﬁnding that the ten-sile strength of the cement-aggregate bond is lower than that of cement paste. Recently, Rao and Prasad  and Gu et al.  found that the tensile strength of the interface between aggregate and mortar was about one third to one half of the tensile strength of the mortar. Mielniczuk et al.  and Jebli et al.  have characterized the behavior of a composite with spherical aggregate using compression
and tensile tests. They showed, at this scale, that the pro-posed models on the macroscopic scale by Eurocode 2 are conﬁrmed to predict behavior at rupture.
In conclusion, all experimental studies to characterize the interface between cement paste and aggregate remain insuﬃcient to assess the behavior law at local scale. In this context, the objective of this study is to determine the me-chanical properties of the interface between the aggregate and the cement paste composite by direct tensile and shear tests.
2 Experimental program
The selected cement is a Portland cement CEM II 32.5 CP2 NF used to prepare all composites with a wa-ter/cement ratio of 0.5.
2.1 Preparation for samples
Natural limestone parallelepipedic aggregates were made with dimensions of 10x10x15 mm3.
In this experimental study, two types of samples whose dimensions are shown in Figure 1, were made:
• For tensile tests, the samples have a thin cement paste layer of 2 mm between two limestone aggregates (Fig. 1a).
• For direct shear tests, the samples are composed of a limestone aggregate and cement paste (Fig.1b).
The samples were prepared using speciﬁc molds adapted to the desired dimensions of the composite. All samples © The Authors, published by EDP Sciences. This is an open access article distributed under the terms of the Creative Commons Attribution
Figure 1. Sample sizes for direct tensile test a) and shear test b)
are demolded after 24 hours of hydration and are imme-diately immersed in water saturated with lime at a tem-perature of 21◦C to prevent the leaching and to decrease concrete shrinkage.
At diﬀerent times of hydration (2, 7, 15, 28 and 90 days), we examine both the direct tensile and the shear bond strengths of the composite by means of speciﬁc devices. The shear tests are conducted for diﬀerent normal stresses. All the tests are designed to characterize mechanical inter-action laws at the local scale of the cement paste-aggregate interface.
To obtain the mechanical properties of the cement paste, mechanical tests were also carried out on cement paste samples of dimensions equal to those of composites.
2.2 Direct tensile test
To perform mechanical tests of direct tensile, experimental devices were designed and manufactured to be adapted to the size and shape of the desired samples. The principle of these tests is simple, but the preparation and implementa-tion should be made carefully. Indeed, each mis-alignment of the supports or in the tilt sample induced parasitic bend-ing which changes the results. Four metal shims with holes are ﬁrst ﬁxed onto the sample as shown in Figure 2. To perform the test, the sample is ﬁxed by placing the metal rods in the holes of shims and of the U-shaped support set on the machine.
Figure 2. Experimental device for direct tensile test
2.3 Direct shear test
This test is among the most diﬃcult tests to be performed on cementitious materials, especially to characterize the
cement paste-aggregate interface due to the lack of appro-priate experimental tools. The objective of our original approach is to access the Mohr-Coulomb law of cement paste-aggregate interface (local cohesion and friction an-gle). To perform this test, experimental devices were de-signed and manufactured in a way that the rupture is lo-cated at the cement paste-aggregate interface. The device consists of two half-boxes, the distance between these two half-boxes is around 0.5 mm to minimize the sample bend-ing. The interface is ﬁxed in the middle of the device with screws. These crews are also used to apply a normal force. Figure 3 illustrates the experimental apparatus in which the sample is placed inside the two half-boxes.
Figure 3. Experimental device for direct shear test
All tests were performed on a "Mechanical Testing System" by imposing a constant loading speed of 0.01 mm/s. Mechanical tests were ﬁlmed with a fast camera Vision Research Phantom V12 (acquisition speed of 10 to 40 thousand pictures per second), to correct the displace-ment during the tests by image correlation.
3 Experimental results
It is proposed to present the experimental results obtained from the direct tensile and shear tests, on cement paste and the composite. For all the tensile and shear tests, it is observed that all the breaks on the composite occur at the cement-aggregate interface (Fig. 4), which represents the weakest zone.
Figure 4. Crack growth at interface during tensile test
3.1 Direct tensile tests
Figure 5 shows the stress evolution as a function of the strain respectively for the composite "cement paste-aggregate" (Fig. 5a) and for pure cement paste (Fig. 5b). Signiﬁcant increase in strengthσr(j) at the beginning of hydration, and a progressive stabilization after three weeks
of hydration for the composite and cement paste is ob-served.
Figure 5. Evolution of the stress vs strain during tensile tests for composite a) and cement paste b)
Figure 6 shows the evolution of the strengthσr(j) in func-tion of hydrafunc-tion time j during tensile tests for cement paste and composite. The results show a similar evolu-tion of the strength, but at each hydraevolu-tion time the cement paste has higher characteristics than the composite. In ad-dition, ratio between composite and cement paste is about 2/3 for the tensile strength. These results tend to conﬁrm that the cement paste-aggregate interface is the weakest zone in composite. An increase of the strain values is also observed with curing, with higher values for the compos-ite than that for the cement paste. Indeed this shows the more "ductile" character of the composite than of the ce-ment paste.
3.2 Direct shear tests
The curves of stress - strain, obtained during direct shear tests (without normal stress), are presented in Figure 7 at diﬀerent hydration times during the ﬁrst 40 days for the cement paste and composite. These ﬁgures show a fast increase in the shear strength and stiﬀness of the samples at the beginning of hydration. We noticed a decrease in the evolution speed of the shear strength after 28 days. With both the shear test and the tensile test, a rapid drop in stress is observed just after it reached its peak. So, an absence of the softening part of the stress-strain curve is observed in macroscopic conventional mechanical behav-ior under shear stress. An increase of the strain values is
Figure 6. Evolution of tensile strength as a function of hydration time during tensile tests for composite and cement paste
also observed in the case of the composite with curing, with lightly higher values of the composite beyond 7 days than that of the cement paste. In this case the crack spreads quickly in the cement-aggregate interface. For the cement paste, breaking is conducted in the same strain value what-ever the time of hydration.
Figure 7. Shear stress-strain curves for composite a) and cement paste b)
The values of strengthτr(j) (MPa) as a function of the hy-dration time j (in days), for the shear test for the cement paste and the composite, are shown on Figure 8. This ﬁg-ure shows a similar increase in strength during hydration time for both types of samples. After the characterization of the eﬀect of hydration time on the shear strength, re-spectively for pure cement paste and for the cement paste-aggregate interface, we focus on the inﬂuence of normal
Figure 8. Evolution of the shear strength as a function of hydra-tion time for the composite and the cement paste
stress on the shear strengths. The samples, at a ﬁxed hy-dration time (40 days), are subjected to direct shear tests at diﬀerent normal stresses. The obtained stress-strain curves are shown in Figure 9 for diﬀerent normal stresses (0, 0.5, 1, 1.5 MPa).
Figure 9. stress-strain curves during shear tests for composite a) and cement paste b) at diﬀerent normal stresses and at 40 days
We noticed that there is a strong dependence of mechanical behavior of composite and cement paste on normal stress. For both samples, an increase in shear strength due to ap-plication of normal stress is noted. The initial tangential modulus also increases in the same way. This evolution of shear strength according to normal stress (Fig. 10) is used to calculate the local friction angle and cohesion accord-ing to the Mohr-Coulomb criterion. We noticed a linear evolution of the shear strength with the increase of normal stress, for both cement paste and composite. The results, presented in Table 1, show that the local cohesionc and
the local friction angleΦ of the paste are greater than that of the composite.
Figure 10. Mohr - Coulomb criterion for the composite and the cement paste at 40 days of hydration
Cement paste Composite
Local cohesionc (MPa) 4.1 2.9
Local friction angleΦ (◦) 54 47
These results are a ﬁrst approach to characterize the me-chanical properties of the interface with the original exper-imental tools. The experexper-imental results showed that the cement-aggregate interface is the weakest zone in com-posite. For both tests the strain values of the composite are higher than those of cement paste. Indeed, the more "ductile character" of the composite compared to the ce-ment paste was more marked for the tensile test than for the shear test. These results at the local scale will improve numerical models (eg CZM) by identifying the parameters to be included in the calculation codes.
 K.M. Alexander, D.J. Gilbert, J. Wardlaw (1968)  S.P. Shah, F.O. Slate, Cement and Concrete Assoc,
London UK (1968)
 G.A. Rao, B.R. Prasad, Cement and Concrete Re-search 32, 253 (2002)
 X. Gu, L. Hong, Z. Wang, F. Lin, Construction and Building Materials 46, 156 (2013)
 B. Mielniczuk, M. Jebli, F. Jamin, M.S. El Youssouﬁ, C. Pelissou, Y. Monerie, Cement and Concrete Re-search 79, 235 (2016)
 M. Jebli, F. Jamin, E. Garcia-Diaz, M. El Omari, M.S. El Youssouﬁ, Cement and Concrete Composites 12, 241 (2016)
Table 1. Local cohesion c and friction angle Φ of the composite and the cement paste at 40 days of hydration